A Study of Water Treatment Chemical Effects on Type I” Pitting Corrosion of Copper Tubes

It is known that one of the causes of pitting corrosion of copper tubes is residual carbon on the inner surface. It was confirmed that type I” pitting corrosion of the copper tube is suppressed by keeping the residual carbon amount at 2 mg/m 2 or less, which is lower than that of the type I’ pitting corrosion, or by removing the fine particles that are the corrosion product of galvanized steel pipes. The developed water treatment chemical was evaluated using three types of copper tubes with residual carbon amounts of 0 mg/m 2 , 0.5 mg/m 2 , and 6.1 mg/m 2 . The evaluation was conducted for three months in an open-circulation cooling water system and compared with the current water treatment chemical. Under the current water treatment chemical conditions, only the copper tube with a residual carbon amount of 6.1 mg/m 2 showed a significant increase in the natural corrosion potential after two weeks, and pitting corrosion occurred. No pitting corrosion and no increase in the natural corrosion potential were observed in any of the copper tubes that were treated with the developed water treatment chemical. In addition, the polarization curve was measured using the cooling water from this field test, and the anodic polarization of two cooling waters was compared. For copper tubes with a large amount of residual carbon, the current density near 0 mV vs. Ag/AgCl electrode (SSE) increased when the developed water treatment chemical was added.


Introduction
Copper has a high thermal conductivity and is easy to process, so it is used for heat exchangers in refrigerators and air conditioning units. Copper tubes are resistant to corrosion in freshwater but may experience pitting corrosion. It has been reported that one of the causes of this pitting corrosion is the effect of the residual carbon on the inner surface of the copper tube [1] [2] [3] [4].
The pitting corrosion of copper tubes is categorized as type I or type II. Type I pitting corrosion is further categorized into two types. One is type I' pitting corrosion when using groundwater, and the other is type I" pitting corrosion when using heat storage or cooling water [5]. To prevent these types of corrosion, it has been proposed that in the case of type I' corrosion, the concentration of free carbonic acid be reduced to less than 15 ppm or the amount of mean residual carbon on the copper tube inner surface (hereafter referred to as "residual carbon amount") be reduced to 5 mg/m 2 or less [6]. On the other hand, type I" is suppressed by reducing the residual carbon amount to 2 mg/m 2 or less, which is lower than that of type I', or by filtering out fine particles that are the corrosion products of the main galvanized steel pipe [7]. However, due to the production cost of copper tubes as industrial products, the development of a water treatment chemical capable of suppressing pitting corrosion even in the presence of residual carbon is desired, rather than removing the residual carbon [8].
In this study, the corrosion suppression effect of the newly developed water treatment chemical was evaluated in a field test of an open-circulating cooling water system using copper tubes with different amounts of residual carbon. In addition, a comparison with a current water treatment chemical was performed by polarization measurement using cooling water from this field test. Table 1 shows the types of test specimens used in the field test. The specimen material was phosphorus deoxidized soft copper tube (JIS H3300 C1220). The residual carbon amount in the tube was controlled to three different levels, 0 mg/m 2 (hereafter referred to as "C_0"), 0.5 mg/m 2 (hereafter referred to as "C_0.5") and 6.1 mg/m 2 (hereafter referred to as "C_6.1"). The C_0 and C_0.5, specimens had an outer diameter of 15.88 mm, wall thickness of 1.0 mm, and length of 200 mm. The C_6.1 specimen had an outer diameter of 15.88 mm, wall thickness of 0.8 mm, and length of 200 mm. They were not subjected to degreasing or other treatments. The test specimens of the field test, which were taken out every month, were cut in half along the length, and the inner surface was inspected. After removing the scale and corrosion products from each specimen with dilute sulfuric acid, the pit depth was measured with a digital microscope (VHX-5000; Keyence). (JIS H3300 C1220). The residual carbon amount in the tube was four types, C_0, C_0.5 and 6.6 mg/m 2 (hereafter referred to as "C_6.6"), 13.0 mg/m 2 (hereafter referred to as "C_13.0"). The C_6.6 and 13.0 specimens had an outer diameter of 15.88 mm, and wall thickness of 0.8 mm. All test specimens were half-cut that had a length of 100 mm that were coated with silicone resin, except for the 1 cm 2 test area on its inner surface. These were degreased before the test using acetone. Figure 1 shows a schematic diagram of the test equipment installed in the cooling tower of the open-circulating cooling water system. There were two refrigerators of the same type, one of which was treated with a newly developed water treatment chemical (hereafter referred to as the "development chemical"), and the other with a current water treatment chemical (hereafter referred to as the "current chemical"). The development chemical was manufactured by Kurita Water Industries. and contained an oxidant-type biofouling control agent, azole-type anti-corrosive agent and phosphonic acid, and the current chemical manufactured by other companies contained a biofouling control agent, an azole-type anti-corrosive agent, and chelating agents. The test was conducted for three months, and the average water quality during the test period is shown in Table 3. Four sets of three types of test specimens were installed in each of the two systems, and the corrosion potential of the specimens was monitored every two weeks with reference to an Ag/AgCl electrode (SSE). For the other three, one was taken out every month for corrosion inspection. The test equipment was designed to circulate water through the test specimen at a flow rate of 0.1 m/s and then return to the cooling tower.      Corrosion products were observed in the test specimens after one month, and it was observed that corrosion products became larger and increase in number over time. Similar to this test, pitting corrosion was reported to occur in copper tubes with residual carbon amount of 3 mg/m 2 or more in a field test of a cooling water system, which confirmed these results [9].    weeks. After that, although it temporarily decreased, it remained at approximately 160 mV vs. SSE, which was a noble value compared to that of the other copper tubes with low residual carbon amount. It has been reported that the potential for pitting corrosion affected by residual carbon is approximately 100 mV vs. SCE (approximately 147 mV vs. SSE in SSE conversion, broken line in Figure   5) [7]. Specimen C_6.1 B reached this potential after two weeks, and pitting was considered to have occurred during this period.    the natural corrosion potential of test water A was more noble than that for test water B. In addition, the current density also showed a difference near 0 mV vs.

Anodic Polarization Curve in Cooling Water
SSE for a residual carbon amount of 6.6 mg/m 2 or more, and the current density in test water A remained higher. Figure 8 shows the relationship between the residual carbon amount and the maximum current density in the anodic polarization measurement. It has been reported that a current density near 0 mV vs. SSE suggests the formation of an oxide film [10]. These results indicated that copper tubes in the test water A were more likely to form an oxide film than those in test water B. Regardless of the residual carbon amount, the current densities of  the anodic polarization curves of both test waters A and B increased significantly from approximately +120 mV vs. SSE. Therefore, under the present measurement conditions, the film breakdown potential of type I" was considered to be approximately +120 mV vs. SSE. In test water B, the natural corrosion potential of 6.1 mg/m 2 reached +180 mV vs. SSE after two weeks, and pitting corrosion appeared. Thus, there was good agreement between this consideration and the field test results.
As described above for the investigation results for the copper tube and the measurement results of the natural corrosion potential, no pitting corrosion and a significant increase in potential were observed in the development chemical regardless of residual carbon amount. It was found that pitting corrosion was greatly affected by the residual carbon amount and the water treatment chemical used. It is currently believed that the pitting corrosion inhibition of this development chemical is due to a composite film consisting of phosphonic acid, an azole type anticorrosive agent contained in the water treatment chemical, and dissolved components in the water [11]. This is still under investigation and will be clarified in the future.

Conclusions
The corrosion suppression effect of the developed water treatment chemical was evaluated in a field test of a cooling water system, and a comparison with a current water treatment chemical was performed by polarization measurements using copper tubes with different amounts of residual carbon. The results were as follows.
1) Regardless of the residual carbon amount, the test specimens with the developed water treatment chemical did not exhibit any pitting corrosion or a significant increase in the natural corrosion potential.
2) No pitting corrosion was observed at the residual carbon amount of 0.5 treatment, but at 6.1 mg/m 2 , a significant increase in natural corrosion potential and the occurrence of pitting corrosion were observed.
3) Regarding the effect of residual carbon amount, regardless of the water treatment chemical, 0 mg/m 2 and 0.5 mg/m 2 showed relatively close behavior, 6.6 mg/m 2 and 13.0 mg/m 2 showed relatively similar behavior, and the polarization behavior tended to be different when the residual carbon amount was 0.5 mg/m 2 or less and 6.6 mg/m 2 or more.

4)
Regarding the difference in water treatment, for copper tubes with a large amount of residual carbon, the current density near 0 mV vs. SSE increased when the developed water treatment chemical was added.
5) Under these measurement conditions, the film breakdown potential of type I" pitting corrosion was considered to be approximately +120 mV vs. SSE.
6) The corrosion inhibition mechanism of the development chemical will be clarified in the future.